| ||Format||Pages||Price|| |
|7||$54.00||  ADD TO CART|
|Hardcopy (shipping and handling)||7||$54.00||  ADD TO CART|
Significance and Use
4.1 This test method is intended as a means for obtaining an extract of mining waste. The extract may be used to estimate the release of certain inorganic constituents of the waste under the laboratory conditions described in this test method. The user is advised to minimize the holding time between sampling and testing if the waste is suspected to contain reactive sulfide minerals.
Note 3: This method is not intended to be used as a kinetic test to simulate weathering of mining wastes. For kinetic testing of mining wastes, refer to Test Method to determine release rates for constituents of interest. For static testing of metal mining ore and mining or mineral processing waste materials, refer to Test Methods .
4.2 The pH of the extraction fluid used in this test method is to reflect the pH of acidic precipitation in the geographic region in which the waste being tested is to be disposed (see ).
4.3 An intent of this test method is for the final pH of the extract to reflect the interaction of the extractant with the buffering capacity of the waste.
4.4 This test method is not intended to provide an extract that is representative of the actual leachate produced from a waste in the field or to produce extracts to be used as the sole basis of engineering design. If the conditions of this test method are not suitable for the test material, USEPA Method 1312 or Test Method may be used.
4.5 This test method has not been demonstrated to simulate actual disposal site leaching conditions.
4.6 This test method produces extracts that are amenable to the determination of both major and minor (trace) inorganic constituents. When minor constituents are being determined, it is especially important that precautions be taken in sample storage and handling to avoid possible contamination of the samples.
4.7 This test method has been tested to determine its applicability to certain inorganic components in the waste. This test method has not been tested for applicability to organic substances, volatile matter (see ), or biologically active samples. This test method has undergone limited testing to determine its reproducibility.
1.1 This test method covers a procedure for the shake leaching of mining waste containing at least 80 % dry solids (≤20 % moisture) in order to generate a solution to be used to determine the inorganic constituents leached under the specified testing conditions that conform to the synthetic precipitation leaching procedure (SPLP).
1.2 This test method calls for the shaking of a known weight of mining waste with acidic extraction fluid of a specified composition, as well as the separation of the liquid phase for analysis. The pH of the extraction fluid is to reflect the pH of acidic precipitation in the geographic region in which the waste being tested is to be disposed.
Note 1: Possible sources of information concerning the pH of the precipitation in the geographic region of interest include state and federal environmental agencies, state universities, libraries, etc. pH values given in USEPA Method 1312, that are 4.2 east of the Mississippi River and 5.0 west of the Mississippi River and are based on acid precipitation maps, are examples of values that can be used. If the pH of the laboratory water is less than the desired pH for the site, do not use this test method; use Practice or Test Method .
Note 2: The method may also be suitable for use in testing of mineral processing waste from metal mining process operations for jurisdictions that do not require the use of Test Method .
1.3 This test method is intended to describe the procedure for performing single batch extractions only. It does not describe all types of sampling, sample preservation, and analytical requirements that may be associated with its application.
1.4 The values stated in SI units are to be regarded as the standard. No other units of measurement are included in this standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.6 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D75/D75M Practice for Sampling Aggregates
D420 Guide for Site Characterization for Engineering Design and Construction Purposes
D653 Terminology Relating to Soil, Rock, and Contained Fluids
D1129 Terminology Relating to Water
D1193 Specification for Reagent Water
D2234/D2234M Practice for Collection of a Gross Sample of Coal
D2777 Practice for Determination of Precision and Bias of Applicable Test Methods of Committee D19 on Water
D3370 Practices for Sampling Water from Flowing Process Streams
D3987 Practice for Shake Extraction of Solid Waste with Water
D5744 Test Method for Laboratory Weathering of Solid Materials Using a Humidity Cell
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
E877 Practice for Sampling and Sample Preparation of Iron Ores and Related Materials for Determination of Chemical Composition and Physical Properties
E1915 Test Methods for Analysis of Metal Bearing Ores and Related Materials for Carbon, Sulfur, and Acid-Base Characteristics
E2242 Test Method for Column Percolation Extraction of Mine Rock by the Meteoric Water Mobility Procedure
ICS Number Code 73.020 (Mining and quarrying)
UNSPSC Code 81102000(Mining engineering)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D6234-13(2020), Standard Test Method for Shake Extraction of Mining Waste by the Synthetic Precipitation Leaching Procedure, ASTM International, West Conshohocken, PA, 2020, www.astm.orgBack to Top